DOI 10.1007/s10948-007-0236-5

**Admixture of an s-Wave Component to the d-Wave Gap**

**Symmetry in High-Temperature Superconductors**

**Albert Furrer**

Received: 10 June 2007 / Accepted: 3 July 2007 / Published online: 3 August 2007 © Springer Science+Business Media, LLC 2007

**Abstract Neutron crystal-field spectroscopy experiments**
in the Y- and La-type high-temperature superconductors
HoBa2Cu3O*6.56*, HoBa2Cu4O8, and La*1.81*Sr*0.15*Ho*0.04*
-CuO4 are reviewed. By this bulk-sensitive technique,
in-formation on the gap function is obtained from the
relax-ation behavior of crystal-field transitions associated with
the Ho3+ ions which sit as local probes close to the
su-perconducting copper-oxide planes. The relaxation data
ex-hibit a peculiar change from a convex to a concave shape
*between the superconducting transition temperature T*cand
*the pseudogap temperature T*∗ which can only be modeled
satisfactorily if the gap function of predominantly d-wave
symmetry includes an s-wave component of the order of 20–
25%, independent of the doping level. Moreover, our results
are compatible with an unusual temperature dependence of
*the gap function in the pseudogap region (T*c*≤ T ≤ T*∗*)*,
i.e., a break up of the Fermi surface into disconnected arcs.
**Keywords High-temperature superconductors**· Gap
symmetry· Pseudogap · Crystal field · Neutron
spectroscopy

**1 Introduction**

Ever since the discovery of high-temperature supercon-ductivity by Bednorz and Müller [1], there has been a debate concerning the symmetry of the superconducting gap function. So far, tunneling measurements are the only

A. Furrer (

)Laboratory for Neutron Scattering, ETH Zurich & PSI Villigen, CH-5232 Villigen PSI, Switzerland

e-mail: albert.furrer@psi.ch

phase-sensitive experiments that probe the sign of the order
parameter [2]. Angle-resolved photoemission spectroscopy
(ARPES) measurements, on the other hand, yield very
di-rect information about the magnitude and the momentum
dependence of the order parameter as well as its evolution
with temperature [3, 4]. Tunneling as well as ARPES
ex-periments indicate that a d*x*2* _{−y}*2 order parameter is the most

plausible candidate to describe the superconducting state in
these systems. However, both techniques are only sensitive
to the surface. As pointed out by Müller [5], the gap
func-tion is different at the surface and in the bulk, thus bulk
ex-periments are indispensable to unambiguously establish the
nature of the gap function. Various experiments probing the
bulk gave evidence for the existence of an s-wave
compo-nent, but the results are partially conflicting. For optimally
doped YBa2Cu3O7, e.g., Raman scattering evidences an
s-wave admixture of 5% [6], thermal conductivity
measure-ments in a rotating magnetic field place a maximum of 10%
based on the shift of the nodal positions from the
princi-pal diagonal directions [7], and nuclear magnetic resonance
experiments report either an s-wave admixture of 20% [8]
or a pure d-wave symmetry [9]. Theoretical work based
*on the t–t**–J model suggests that d-wave pairing prevails*
close to optimum doping, whereas s-wave-like pairing is
possible in the under- and over-doped regimes [10].
Doping-dependent bulk experiments are, therefore, extremely useful
to shed light on this issue. The present work deals with such
an investigation for underdoped and optimally doped

*high-T*ccompounds studied by neutron crystal-field spectroscopy
experiments.

Neutron crystal-field spectroscopy is a powerful
experi-mental tool to probe the bulk properties of high-temperature
superconductors. It has been applied in the past mainly to
detect the doping, isotope, and pressure dependence of the
*pseudogap temperature T*∗. In principle, information on the

nature of the gap function can be obtained as well,
pro-vided that the experimental data sets are sufficiently
com-plete. We reviewed the available data sets in the literature
and found the necessary conditions fulfilled for some
*un-derdoped and optimally doped La- and Y-based high-T*c
compounds. We analyzed the corresponding data sets and
found evidence for a 20–25% s-wave admixture to the
dom-inant d-wave gap function, independent of the doping level.
Moreover, our analysis supports the unusual temperature
dependence of the gap function in the pseudogap region
*(T*c*≤ T ≤ T*∗) as evidenced by ARPES measurements in
Bi2Sr2CaCu2O8*+x*[11].

**2 Neutron Crystal-Field Spectroscopy**

The principle of neutron crystal-field spectroscopic
investi-gations of the crystal-field interaction in rare-earth based
high-temperature superconductors was described in a
re-cent review article [12]. By this technique, transitions
be-tween different crystal-field levels associated with the
rare-earth ions can be directly measured. In the normal metallic
state, the excited crystal-field levels interact with phonons,
spin fluctuations and charge carriers, which limit the
life-time of the excitation, thus the observed crystal-field
tran-sitions exhibit line broadening. The interaction with the
charge carriers is by far the dominating relaxation
mecha-nism [13]. The corresponding intrinsic linewidth Wn*(T )*
in-creases almost linearly with temperature according to the
well-known Korringa law [14], i.e., Wn*(T )∼ T . In the*
pseudogap as well as in the superconducting state,
how-ever, the pairing of the charge carriers creates an energy gap

*Δ***k** **in the single-electron spectral function (k is the wave**
*vector), thus crystal-field excitations with energy <2Δ***k**do
not have enough energy to span the gap. Consequently,
the interaction with the charge carriers is suppressed,
*and for an isotropic gap function Δ***k** *= Δ, the intrinsic*
*linewidth is given by W*s*(T )= W*n*(T )· exp[−Δ/kBT*].
*This means that W*s*(T* * T*c*, T*∗*)*≈ 0, and line
*broad-ening sets in just below T*c *(or T*∗) where the
supercon-ducting gap (or the pseudogap) opens. For anisotropic gap
functions, the situation is more complicated, since
cer-tain relaxation channels exist even at the lowest
tempera-tures [15].

Recently, Häfliger et al. [16] presented detailed
consid-erations concerning the analysis of neutron crystal-field
re-laxation data with respect to the nature of the gap
func-tion. As mentioned above, a crucial point in such
analy-ses is the availability of a sufficient number of
relax-ation data over a large temperature range, notably for the
*pseudogap region T*c*≤ T ≤ T*∗, so that the subtle but
rel-evant features of the relaxation behavior can
unambigu-ously be assessed. So far, such complete data sets are

**Fig. 1 Temperature dependence of the intrinsic linewidth of the**
lowest crystal-field ground-state transition in HoBa2Cu3O*6.56* **(a),**

HoBa2Cu418O8 **(b), and La***1.81*Sr*0.15*Ho*0.04*Cu18O4**(c). The dashed**

line corresponds to the linewidth in the normal state as expected from the Korringa law

only available for underdoped HoBa2Cu3O*6.56*[17], slightly
underdoped HoBa2Cu418O8 [18], and optimally doped
La*1.81*Sr*0.15*Ho*0.04*Cu18O4 [19] as shown in Figs.1(a–c).
For all three compounds, the temperature dependence of the
*intrinsic linewidth W (T ) behaves in a common and *
charac-teristic way:

*(i) T* *≤ T*c: The linewidth is very small, but a slight
*en-hancement is observed upon approaching T*c.

*(ii) T* *≥ T*∗: The linewidth increases linearly as expected
*for the normal state, so that we identify T*∗ with the
temperature where the pseudogap opens.

*(iii) T*c *≤ T ≤ T*∗: There is a sudden increase of the
*linewidth just above T*c. Then, with increasing
*tem-perature, the slope dW/dT is slightly reduced, but*
*increases again upon approaching T*∗. The

tempera-ture dependence of the linewidth obviously exhibits a change from a convex to a concave shape in the pseudo-gap region.

The only differences between the three data sets are the
*dif-ferent sizes of the characteristic temperatures T*c*and T*∗. It
is, therefore, useful to express the relaxation data in reduced
*units, i.e., the temperature T in units of T*∗and the linewidth

*W (T )in units of W (T*∗*)*as visualized for the relevant
tem-perature range 0*≤ T ≤ T*∗in Figs.2(b–d).

**3 Analysis of the Relaxation Data**

We now proceed to analyze the relaxation data in terms of
different gap functions. The model calculations were based
on the procedure described in Ref. [16]. For the
tempera-ture dependence of the gap amplitude, we used the
*expres-sion Δ(T )= Δ(0) · [1 − (T /T*∗*)A] with A = 4 [*3], and
*the maximum gap amplitude was set to Δ*max*/ k*B*= 2T*∗

which is a realistic value for the compounds under
consider-ation. Figure2(a) shows some calculations for an s-wave,
a d-wave (d* _{x}*2

*2), and a mixed (s25%+ d75%)-wave gap function. It can readily be seen that none of these mod-els is able to explain the observed linewidth behavior dis-played in Figs.2(b–d). The s-wave model reproduces the*

_{−y}*low-temperature behavior up to T*c quite well, but it fails completely at high temperatures. The d-wave model is inad-equate at both low and high temperatures. The mixed (s +d)-wave model has similar deficiencies. In particular, the

*be-havior around T*c

*where the slope of W (T )/W (T*∗

*)*turns from being convex to concave cannot be reproduced by any of the above models. This is due to the neglect of the tem-perature dependence of the gap function in the pseudogap region. According to ARPES experiments performed for un-derdoped Bi2Sr2CaCu2O8

*+x*[11], the pseudogap opens up at different temperatures for different points in momentum space as sketched in Fig.3. Below T∗, there is a break up of the Fermi surface into disconnected arcs, which then shrink

**Fig. 2 Temperature**

dependence of the linewidth of
low-energy crystal-field
transitions in high-temperature
superconductors in reduced
**units. (a) Model calculations for**
different types of gap functions
**(see text). (b–d) Relaxation data**
derived for HoBa2Cu3O*6.56***(b),**

HoBa2Cu418O8**(c), and**

La*1.81*Sr*0.15*Ho*0.04*Cu18O4**(d).**

**The lines in (b–d) denote**
least-squares fits on the basis of
a mixed (s+ d)-wave gap
function including the

occurrence of gapless arcs of the
Fermi surface in the pseudogap
*region (T*c*< T < T*∗*)*as

described in the text

**Fig. 3 Schematic illustration of**
the temperature evolution of the
Fermi surface in the pseudogap
*region (T*c*≤ T ≤ T*∗). The

*d-wave node below T*c*(left*

*panel) becomes a gapless arc*
*above T*c*(middle panel) which*

expands upon increasing the
temperature to form the full
*Fermi surface at T*∗*(right*
*panel)*

**Table 1 Gap parameters**
resulting from the least-squares
fitting procedure applied to the
crystal-field relaxation data
displayed in Figs.2(b–d)

*T*c[K] *T*∗[K] *Δ*s[meV] *Δ*d[meV] *Δ*max[meV]

HoBa2Cu3O*6.56* 60 250 *8.6± 1.2* *28.0± 2.1* *36.6± 3.3*

HoBa2Cu418O8 79 231 *9.3± 0.9* *28.5± 1.6* *37.8± 2.5*

La*1.81*Sr*0.15*Ho*0.04*Cu18O4 32 70 *2.4± 0.4* *7.7± 0.7* *10.1± 1.1*

with decreasing temperature before collapsing to the point
*nodes of the d-wave component below T*c. This unusual
temperature evolution of the pseudogap opens additional
*re-laxation channels in crystal-field linewidth studies above T*c.
Indeed, model calculations including the presence of such
gapless arcs produce relevant modifications of the linewidth
*for T*c*≤ T ≤ T*∗as visualized in Fig.2(a); in particular, the
observed change of the linewidth from a convex to a
*con-cave temperature dependence around T*c can be nicely
re-produced for a mixed (s+ d)-wave gap function, but not for
a pure d-wave gap function.

We performed a least-squares fitting procedure to the relaxation data displayed in Figs. 2(b–d) on the basis of a mixed (s+ d)-wave gap function including the gapless arc features of the Fermi surface in the pseudogap region

*(T*c*≤ T ≤ T*∗*)*. Since the latter effect was only observed
at a few selected temperatures [11], we assumed a linear
evolution of the gapless arcs with temperature. The only
*fit-ting parameters were the amplitudes Δ*s *and Δ*d of the
s-and d-wave components, respectively. The temperature
evo-lution of the linewidths resulting from the least-squares
fit-ting procedure are in good agreement with the
experimen-tal data as shown in Figs.2(b–d). The corresponding model
parameters are listed in Table 1. We recognize that the
s-wave admixture is independent of the doping level, and the
maximum gap amplitudes are consistent with the
*expecta-tion Δ*max*/ k*B*≈ 2T*∗.

**4 Concluding Remarks**

In conclusion, our analyses of bulk-sensitive crystal-field
relaxation experiments on high-temperature
superconduc-tors give two important results. First, we gave evidence
that the theoretically predicted [20] and for underdoped
Bi2Sr2CaCu2O8*+x* observed [11] gapless arcs of the Fermi
surface are also present in the Y- and La-based
high-temperature superconductors, thereby being presumably a
generic feature of all copper-oxide perovskites. Secondly,
there is evidence for an admixture of an appreciable
s-wave component of the order of 20–25% to the
predom-inant d-wave gap function in both Y- and La-based

*high-T*c superconductors. In fact, for orthorhombic symmetry
both the s- and d-wave pair states belong to the same
ir-reducible representation [21], thus an admixture of these

two states is allowed. Recent angle-resolved electron
tun-neling experiments in YBa2Cu3O7 report similar results,
namely a 17% s-wave admixture to the d-wave gap
func-tion [22]. Moreover, the gap values listed for the
La-based compound in Table 1 are in good agreement with
the results of recent in-plane magnetic-field
penetration-depth measurements in La*1.83*Sr*0.17*CuO4 by muon-spin
*rotation experiments which gave Δ*s*= 1.57(8) meV and*

*Δ*d*= 8.2(1) meV [*23]. A subsequent theoretical study
con-firmed these findings by calculations based on a two-band
model [24].

**Acknowledgement** The author is very much indebted to K.A.
Mü-ller for stimulating discussions.

**References**

**1. Bednorz, J.G., Müller, K.A.: Z. Phys. B 64, 189 (1986)**
**2. Tsuei, C.C., Kirtley, J.R.: Rev. Mod. Phys. 72, 969 (2000)**
3. Ding, H., Yokoya, T., Campuzano, J.C., Takahashi, T., Randeria,

M., Norman, M.R., Mochiku, T., Kadowaki, K., Giapintzakis, J.:
**Nature 382, 51 (1996)**

4. Mesot, J., Norman, M.R., Ding, H., Randeria, M., Campuzano,
J.C., Paramekanti, A., Fretwell, H.M., Kaminski, A., Takeuchi, T.,
Yokoya, T., Sato, T., Takahashi, T., Mochiku, T., Kadowaki, K.:
**Phys. Rev. Lett. 83, 840 (1999)**

**5. Müller, K.A.: Phil. Mag. Lett. 82, 279 (2002)**

6. Limonov, M.F., Rykov, A.I., Tajima, S., Yamanaka, A.: Phys. Rev.
**Lett. 80, 825 (1998)**

7. Aubin, H., Behnia, K., Ribault, M., Gagnon, R., Taillefer, L.: Phys.
**Rev. Lett. 78, 2624 (1997)**

**8. Stern, R., Mali, M., Roos, J., Brinkmann, D.: Phys. Rev. B 51,**
15478 (1995)

**9. Bulut, N., Scalapino, D.J.: Phys. Rev. Lett. 67, 2898 (1991)**
**10. Wheatley, J., Xiang, T.: Solid State Commun. 88, 593 (1993)**
11. Norman, M.R., Ding, H., Randeria, M., Campuzano, J.C., Yokoya,

T., Takeuchi, T., Takahashi, T., Mochiku, T., Kadowaki, K.,
**Gup-tasarma, P., Hinks, D.G.: Nature 392, 157 (1998)**

**12. Furrer, A.: Struct. Bond. 114, 171 (2005)**
**13. Boothroyd, A.T.: Phys. Rev. B 64, 066501 (2001)**
**14. Korringa, J.: Physica (Utrecht) 16, 601 (1950)**

15. Boothroyd, A.T., Mukherjee, A., Murani, A.P.: Phys. Rev. Lett.
**77, 1600 (1996)**

16. Häfliger, P.S., Podlesnyak, A., Conder, K., Pomjakushina, E.,
**Fur-rer, A.: Phys. Rev. B 74, 184520 (2006)**

17. Rubio Temprano, D., Mesot, J., Conder, K., Janssen, S., Mutka,
**H., Furrer, A.: J. Supercond. 13, 727 (2000)**

18. Rubio Temprano, D., Mesot, J., Janssen, S., Conder, K., Furrer,
**A., Mutka, H., Müller, K.A.: Phys. Rev. Lett. 84, 1990 (2000)**
19. Rubio Temprano, D., Conder, K., Furrer, A., Mutka, H., Trounov,

**V., Müller, K.A.: Phys. Rev. B 66, 184506 (2002)**
**20. Wen, X.G., Lee, P.A.: Phys. Rev. Lett. 76, 503 (1996)**

21. Annett, J.F., Goldenfeld, N.D., Renn, S.R.: In: Ginsberg, D.M. (ed.) Physical Properties of High-Temperature Superconductors II, p. 571. World Scientific, Singapore (1990)

22. Smilde, H.J.H., Golubov, A.A., Ariando, G., Rijnders, G.,
Dekkers, J.M., Harkema, S., Blank, D.H.A., Rogalla, H.,
**Hilgenkamp, H.: Phys. Rev. Lett. 95, 257001 (2005)**

23. Khasanov, R., Shengelaya, A., Maiuradze, A., La Mattina, F.,
Bussmann-Holder, A., Keller, H., Müller, K.A.: Phys. Rev. Lett.
**98, 057007 (2007)**

24. Bussmann-Holder, A., Khasanov, R., Shengelaya, A., Maisuradze,
**A., La Mattina, F., Keller, H., Müller, K.A.: Europhys. Lett. 77,**
27002 (2007)